Three Novel Phases in the Sm-Co-Ga System. Syntheses, Crystal and Electronic Structures, and Electrical and Magnetic Properties
YongZhong Jia; Claude Belin; Monique Tillard; Laurence Lacroix-Orio; David Zitoun; GuoHua Feng; Inorganic Chemistry 46 (2007) 4177–4186; doi:10.1021/ic0700755

data_4308096
_publ_contact_author_address
;
Institut Charles Gerhardt  UMR 5253
AIME, CC15
Universit\'e de Montpellier II
Sciences et Techniques du Languedoc
2 Place Eug\`ene Bataillon 
34095 Montpellier C\'edex 5
France
;
_publ_contact_author_email       mtillard@univ-montp2.fr
_publ_contact_author_fax         330467143304
_publ_contact_author_name        'Monique TILLARD / Claude BELIN'
_publ_contact_author_phone       330467144897
_publ_section_title
;
Three Novel Phases in the Sm-Co-Ga System. Syntheses, Crystal and
Electronic Structures, and Electrical and Magnetic Properties
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              4177
_journal_page_last               4186
_journal_paper_doi               10.1021/ic0700755
_journal_volume                  46
_journal_year                    2007
_chemical_formula_moiety         'Co3 Ga16 Sm4'
_chemical_formula_sum            'Co3 Ga16 Sm4'
_chemical_formula_weight         1893.75
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           123
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            1
_cell_length_a                   6.0620(5)
_cell_length_b                   6.0620(5)
_cell_length_c                   11.1495(9)
_cell_measurement_reflns_used    6873
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      32.26
_cell_measurement_theta_min      3.36
_cell_volume                     409.72(6)
_computing_cell_refinement       'CrysAlisRed 171 Oxford Diffraction, 2004'
_computing_data_collection       'CrysAlis 171 Oxford Diffraction, 2004'
_computing_data_reduction        'CrysAlisRed 171 Oxford Diffraction, 2004'
_computing_molecular_graphics    'ORTEP-3 for Windows v.1.075, Farrugia 2002'
_computing_publication_material  'WinGX, Farrugia 1999'
_computing_structure_refinement  'SHELXL-97, Sheldrick, 1997'
_computing_structure_solution    'SHELXS-97, Sheldrick, 1997'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.961
_diffrn_measured_fraction_theta_max 0.961
_diffrn_measurement_device_type  'Oxford Diffraction Xcalibur CCD'
_diffrn_measurement_method       'omega scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0441
_diffrn_reflns_av_sigmaI/netI    0.0158
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            6873
_diffrn_reflns_theta_full        32.32
_diffrn_reflns_theta_max         32.32
_diffrn_reflns_theta_min         3.36
_diffrn_standards_decay_%        0
_exptl_absorpt_coefficient_mu    42.768
_exptl_absorpt_correction_T_max  0.175
_exptl_absorpt_correction_T_min  0.017
_exptl_absorpt_correction_type   numerical
_exptl_crystal_colour            grey
_exptl_crystal_density_diffrn    7.675
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       platelet
_exptl_crystal_F_000             825
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.14
_exptl_crystal_size_min          0.06
_refine_diff_density_max         2.017
_refine_diff_density_min         -2.011
_refine_diff_density_rms         0.343
_refine_ls_extinction_coef       0.0057(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.328
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     28
_refine_ls_number_reflns         474
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.328
_refine_ls_R_factor_all          0.0273
_refine_ls_R_factor_gt           0.0262
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0176P)^2^+5.1318P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0626
_refine_ls_wR_factor_ref         0.0630
_reflns_number_gt                459
_reflns_number_total             474
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic0700755-file003_3.cif
_cod_data_source_block           SmCo0.75Ga4
_cod_database_code               4308096